Access the full text.
Sign up today, get DeepDyve free for 14 days.
The paper presents the results of investigation of the structure of porous condensates of Ag-NaCl and Cu- NaCl composition; chemical and phase compositions and dimensions of nanoparticles, produced from the vapour phase by EBPVD method. Silver and copper nanoparticles in a porous matrix, when removed from vacuum, oxidize in air to lower oxides, and have considerable sorption capacity relative to oxygen and moisture. Heating in air is accompanied by lowering of porous condensate mass, primarily, due to desorption of physically sorbed moisture, as well as afteroxidation to higher oxides due to physically adsorbed oxygen. At copper concentrations up to 10 at.%, sorption capacity of the condensate is greatly enhanced, that is attributable to presence of very fine nanoparticles. Increase of copper concentration in the condensate is accompanied by lowering of sorption capacity of nanoparticles with respect to oxygen, and, therefore, also change of phase composition. In addition to concentration change, phase composition of nanoparticles can be also controlled by heat treatment of the initial condensate produced at low condensation temperatures. Silver and copper nanoparticles can be converted into stable colloidal systems. Keywords: EBPVD, porous condensate, silver and copper nanoparticles, phase composition. 1. Introduction Among the currently produced nanomaterials for medical applications, preparations with silver and copper nanoparticles attract special attention. It is known that silver has stronger antimicrobial properties than does penicillin, biomycin and a number of other antibiotics, having a devastating effect on antibiotic resistant bacterial strains [1-3]. Moreover, silver aquasol has a synergic effect, extending the term of action of some antibiotics many times [1, 4, 5]. The antiseptic effect is achieved at application of a smaller quantity of antibiotic. It is also shown that nanosilver stimulates the immune system, stabilizes the metabolism in the living body and disinfects about 100 species of dangerous bacteria, viruses and fungi [6, 7], while the antibacterial spectrum of any antibiotic extends to 5-10 strains of microorganisms. Here, oxides of these metals are better antibacterial agents, degree of metal oxidation playing a significant role [7-9]. It is found [10-12] that in addition to silver, nanoparticles of copper and copper oxide also exert a pronounced antibacterial effect on gram-positive and gram-negative bacteria. Copper itself is a vital (i.e. essential) element for living organisms. In particular, it is a cofactor of more than 20 enzyme systems that provide both the mammalian and human multiple processes of vital activity, and the body's resistance to bacterial infections and other invasions. Although copper has less pronounced antiseptic properties than silver, it can significantly enhance the effect of silver preparations [6, 13]. Nanoparticles, produced practically by all the methods, are in a metastable non-equilibrium state. This circumstance complicates their study and use in nanotechnology to create stably operating devices. On the other hand, the non-equilibrium of the system enables conducting new, unusual and hardly predictable chemical transformations. For small particles, specific size effects are most strongly manifested, where irregular dependencies of properties on particle size prevail. The degree of activity of the nanoparticle, depending on its size, is due to its changing properties when interacting with the adsorbed reagent . The main adsorbed reagent for metal nanoparticles is oxygen. Further development and creation of medicines based on silver and copper nanoparticles require selecting a method for synthesis of nanoparticles that would ensure production of various nanomaterial compositions based on these metals with a specified content of the necessary structural components. In most cases, the physical methods for synthesizing nanoparticles are based on physical processes of evaporation or atomizing of substances by highly concentrated energy sources followed by deposition of the vapor phase (atomic-molecular beams) in vacuum, or atmosphere of inert or active gases. In this respect, the method of electron beam evaporation and deposition of materials in vacuum opens up wide possibilities [15, 16]. The idea of using this approach is the possibility of simultaneous evaporation and deposition of mixed molecular flows of two substances onto a substrate. By lowering the temperature of the substrate, it is possible to ensure the limitation of diffusion mobility of atoms in the solid state and, thereby, to create conditions for the formation of a composite structure with the necessary element ratios and their dispersion. Water-soluble substances, for example sodium chloride [17-19], are used as the main component (matrix), that gives an advantage in further use of these substances for the preparation of colloidal solutions. This paper presents the results of studying the processes of physical synthesis of silver and copper nanoparticles by molecular beams, their thermal stability at interaction with air oxygen, and the method of conservation of deposited particles in a salt matrix designed to store particles in an un-aggregated state for further use in medicine. 2. Experimental procedure A metal ingot and compacted NaCl cylinder were placed into cylindrical water–cooled crucibles of 50 mm diameter, located side-by-side. A vacuum of 1.3 – 2.6 × 10-2 Pа was created in the reaction chamber. Both the materials were heated in the crucibles by electron beam gun up to complete melting. This resulted in formation of a mixed vapor flow of metal and NaCl particles, which condensed on a water-cooled substrate at the temperature of 40-50 °C. After bleeding air and complete unsealing of the chamber, the condensate was scraped off the substrate, and the deposited nanoparticles were studied both in dry condensate and in a colloidal solution after their dissolution. X-ray diffraction (XRD) data for carrying out qualitative phase analysis (including lattice parameters refinement and crystal structure refinement) were collected with DRON-3 automatic diffractometer (CuKα radiation). The diffraction patterns have been obtained in a discrete mode under the following scanning parameters: observation range 2θ = (20–120)°, step scan of 0.05°, and counting time per step at 3 s. The microstructure of the condensate and its elemental content were examined with both the CamScan (Cambridge CamScan SEM, UK) scanning electron microscope (SEM) and the INCA- 200 energy-dispersive X-ray imager (Oxford Inca Energy 200 EDS system, UK) and the transmission electron microscopy (TEM) method using H-800 microscope (Hitachi, Japan) at an accelerating voltage of 100 kV. The air oxidation of metallic nanoparticles placed in the salt matrix was studied using a thermogravimetric analyzer TGA-7 (Perkin Elmer, USA) (heating/cooling at 10 °C / min to 650 °C). The size of the nanoparticles in the colloidal system was studied by dynamic light scattering (DLS) [20, 21] using the Zeta Sizer-3000 laser correlation spectrometer (Malvern, UK). 3. Investigation results and discussion 3.1. Deposition of Cu-NaCl and Ag-NaCl condensates on the substrate Condensate synthesis was performed in the work by vacuum deposition of mixed molecular flows of metal and salt particles on the substrate by the technological schematic shown in Fig. 1. Realization of this schematic allows producing on a substrate, heated up to < 0.3 T , the initial condensate of salt with embedded metal nanoparticles and microstructure with open micro- and nanosized porosity [22, 23]. Fig. 1. Process schematic of mixing the vapour flows of salt (NaCl) and metal (Ag or Cu) in vacuum and their Studying the transverse cleavage of porous Cu- deposition on a stationary water-cooled NaCl condensate by EDS method showed a substrate with temperature T . S uniform distribution of elements (copper, sodium, chlorine and oxygen) across the condensate thickness (Fig. 2), that is indicative of maintaining a constant ratio of evaporation rates for individual components of the vapour flow during the entire technological process. (a) (b) Cu O Na Cl Spectrum wt % Spectrum 1 21.0 4.0 27.0 48.0 Spectrum 2 20.0 4.0 27.5 48.5 Spectrum 3 19.2 4.0 27.6 49.2 Spectrum 4 14.6 4.1 31.1 50.2 Spectrum 5 19.8 4.0 27.3 49.0 (c) (d) Fig. 2. Transverse cleavage microstructure (a), element distribution across the thickness (b) and local element analysis (c, d) of Cu-NaCl condensates produced on a water-cooled copper substrate with 40–50 °С temperature. In (a) substrate is on the left, in (c) substrate is below. 3.2. Deposited Cu-NaCl condensate Results of EDS analysis are indicative of presence in Cu-NaCl samples of a certain quantity of oxygen, adsorbed by metal nanoparticles (Figs. 2, 3). Atomic ratio of oxygen to copper content (O/Cu index) in the condensate decreases both at increase of copper content, as at increase of substrate temperature (Fig. 3). A set of data of EDS analysis, scanning electron microscopy of thin chips and XRD studies indicate Fig. 3. Dependence of O/Cu index on the presence of a fine nanoscale substance in the copper content in the condensates of Cu- initial Cu-NaCl condensates (the size of individual NaCl composition, produced at different particles is about 20 nm), whose phase temperatures T : 40 °C and 200 °C. composition corresponds to a mixture of NaCl and Cu O (Figs. 4, 5, Table 1). It should be noted that NaCl lattice period for all the samples studied within the error, corresponds to the lattice period of pure common salt a = 0.5640(2) nm. (a) (b) Fig. 4. Microstructure (a) and electron diffraction pattern (b) of initial Cu-NaCl condensates. Analysis of the above data is indicative of the fact that at breaking the vacuum in the chamber the phase composition of initial condensates is mainly determined by the degree of aggregation of nanoparticles, both in the mixed vapour flow and at their condensation on the substrate (Table 1). So, at a small content of copper (up to ≈ 20 wt %), and, hence at low probability of nanoparticle aggregation, the condensate contains Cu O oxide. At average copper content (≈ 20 – 30 wt %) the condensate predominantly contains a mixture of Cu O and CuO phases, alongside NaCl. And, finally, because of the high probability of nanoparticle aggregation at a high content of copper (≈ 30 – 50 wt %) the fraction of coarser particles increases, and CuO and Cu phases co- exist with Cu O phase. Fig. 6. Kinetics of relative change of the mass Fig. 5. Diffractograms of Cu-NaCl condensate of crushed Cu-NaCl condensate in the initial condition and after annealing at (13.7 wt % Cu) at two cycles of heating and 400 °С on air (phase designation: Cu O, Cu, CuO, balance is NaCl). cooling in air. Therefore, at loss of vacuum in the Table 1 chamber physical adsorption of Phase composition of initial Cu-NaCl condensates oxygen by open surface of active nanoparticles of copper, embedded Cu, wt % Phase composition into the micro- and nanoscale pores 13.7 NaCl (86) + Cu O (10) + CuO (4) of the salt matrix, takes place with formation of Cu O and CuO 23.0 NaCl (77) + Cu O (23) oxides. Coarsening of particles, 26.0 NaCl (76) + Cu O (24) occurring at increase of copper 27.5 NaCl (72) + Cu O (28) concentration in the condensate, leads to individual metal particles 30.0 NaCl (70) + Cu O (27) + CuO (3) consisting of a copper nucleus 32.6 NaCl (67) + Cu O (23) + CuO (5) + Cu (5) coated by an oxide shell. 33.1 NaCl (67) + Cu O (23) + CuO (4) + Cu (6) Heat treatment of the initial 47.1 NaCl (53) + Cu O (32) + CuO (8) + Cu (7) components significantly affects T = 30–50°С, condensate thickness of 125–200 μm. s the phase composition (Table 2). Phase content, wt %, is given in brackets It is shown that increase of the Table 2 temperature of initial condensate treatment promotes acceleration of diffusion processes in Phase content of Cu-NaCl condensate the material, leading to afteroxidation of copper (13.7 wt % Cu) after its heat treatment particles (from Cu O to CuO). The oxidation Heat treatment Phase composition process was studied in detail by the method of gravimetric analysis by the kinetics of relative NaCl (86) + Cu O (10) + Initial change of mass of porous Cu-NaCl condensate CuO (4) (13.7 wt % Cu) at heating up to 650 °C and 300 °C, 1h NaCl (85) + CuO (15) cooling in air (Fig. 6). 400 °C, 1h NaCl (86) + CuO (15) As a result it was shown that with increase of Phase content, wt %, is given in brackets. temperature (at heating at the rate of 10 °C/min) lowering of porous condensate mass occurs right up to 400 °C temperature, due to removal from it of water H O, intercrystalline moisture and OH hydroxyl groups. Further increase of temperature (above 400 °C), is accompanied by a slight increase of porous condensate mass due to afteroxidation of Cu O to CuO by air oxygen (Fig. 2). At heating to about 650 °C, just CuO is present in the condensate, so that further heating cycles are not accompanied by any changes (Fig. 6). It is obvious that annealing in air for one hour at the temperature of 300 °C, ensures running of the process of Cu O afteroxidation with formation of CuO oxide in the condensate (Table 2). With increase of copper content (22.1 wt %) in the condensate, the fraction of adsorbed moist air decreases due to increase of the size of nanoparticles and reduction of their activity (Fig. 7, curve 1). Due to a greater content of Cu O in the initial sample with 22.1 wt % Cu (Table 1), its afteroxidation requires more oxygen. Therefore, after 200 °C, a considerable increase of the mass of condensate with 22.1 wt % Cu is observed right up to 650 °C, Fig. 7. Kinetics of oxidation of Cu-NaCl (Fig. 7, curve 1). Partial afteroxidation with condensates (22.1 wt % Cu) at two cycles of formation of a mixture of Cu O and CuO heating and cooling in air, depending on occurs already during annealing (with annealing temperature T : 1 – initial, 2 – an temperature rise). And, therefore, less oxygen 200 °С, 10 min., 3 – 400 °С, 13 min., 4 – is required for afteroxidation of remaining 650 °С, 5 min. Cu O (Fig. 7, curves 2, 3) and sample growth decreases. And, finally, annealing at the temperature of 650 °C for 5 minutes leads to complete afteroxidation of Cu O phase to CuO (Fig. 7, curve 4), and there is no growth. Thus, a comprehensive study of Cu-NaCl condensates showed that after breaking vacuum in the chamber the condensate deposited on the substrate, in addition to NaCl, also contains a mixture of Cu O and/or CuO oxides, the ratio of which is determined both by concentration of the initial mixture and temperature modes of synthesis and heat treatment. 3.3. Deposited Ag-NaCl condensate According to the data of X-Ray phase and TEM analyses, all the synthesized and heat- treated condensates are two-phase and contain a mixture of NaCl and silver (Figs. 8, 9, Table 3). TEM study of thin chips of porous Ag- NaCl condensate revealed presence of a nanoscale substance of 10 nm size (Fig. 9). It should be noted that according to XRD data, the silver lattice periods at these Fig. 8. Diffractograms of Ag-NaCl condensate transformations are constant within the error, in the initial condition and after annealing at while the period of NaCl lattice increases T = 300 and 650 °С (phase designation: Ag, an significantly at annealing (Table 3, Fig. 10). balance is NaCl). (a) (b) Fig. 9. Microstructure (a) and electron diffraction pattern (b) of initial Ag-NaCl condensates. To clarify the nature of variation of the lattice period (Fig. 10), the crystalline lattice of sodium chloride was determined more precisely for Ag-NaCl condensate in the initial condition and after its annealing at 650 °C (Table 4). Table 3 Characteristics of the phases according to XRD analysis of Ag-NaCl Ag NaCl Sample Phase composition Lattice Grain sizes, D, Lattice parameter, a, nm nm parameter, a, nm Varying the substrate temperature, T Initial Ag (45) + NaCl (55) 0,4088(2) 6(1) 0,5636(2) 200 °C Ag (48) + NaCl (52) 0,4084(2) 5(1) 0,5630(2) 400 °C Ag (45) + NaCl (55) 0,40859(3) 14(1) 0,56368(3) Pounded powder mixture Pounded Ag (50) + NaCl (50) 0,40878(7) 8(1) 0,56368(8) Varying the annealing temperature, T Initial Ag (45) + NaCl (55) 0,4085(2) 9(1) 0,5628(4) 100 °C 1h Ag (47) + NaCl (53) 0,4086(2) 9(1) 0,5633(1) 200 °C 1h Ag (47) + NaCl (53) 0,4088(1) 10(1) 0,5636(1) 300 °C 1h Ag (47) + NaCl (53) 0,40859(3) 15(2) 0,56378(3) 400 °C 1h Ag (45) + NaCl (55) 0,40861(1) 25(2) 0,56391(6) 650 °C 1h Ag (62) + NaCl (38) 0,40859(1) coarse-grained 0,56412(3) Obtained results (Table 4) show that a substitutional solid solution of Na Ag Cl forms on the 0.98 0.02 substrate surface at interaction of molecular flows of salt and silver. During annealing of Ag- NaCl condensate, silver precipitates from this solid solution lattice, and at 650 °C salt is present in the annealed condensate already in its initial condition. Table 4 Crystal data for NaCl compounds existing in the initial Ag-NaCl composite and after its annealing T at 650 °C Atom Site Site occ. X y z Initial Ag-NaCl Na 4a 0.98(1) 0 0 0 Ag 4a 0.02(1) 0 0 0 Cl 4b 1.00(1) 0.5 0.5 0.5 Space group Fm3m (no. 225) Lattice parameter, a, nm 0.5627(2) Independent reflections 15 2 -2 Total isotropic B factor, nm B = 3.28(2)·10 Reliability factor R = 0.053 Annealing at 650 °C Na 4a 1.00(1) 0 0 0 Cl 4b 1.00(1) 0.5 0.5 0.5 Space group Fm3m (no. 225) Lattice parameters, a, nm 0.56391(3) Independent reflections 15 2 -2 Total isotropic B factor, nm B = 1.49(1)·10 Reliability factor R = 0.043 Average grain sizes of Ag phase were determined from line broadening using the classical Williamson–Hall method. The Williamson-Hall graphs have been plotted as dependencies of scaled broadening of Bragg’s reflections β (2θ ) cosθ b * (2θ )= Fig. 10. Dependence of NaCl lattice period on scattering vector S=(2sinθ)/λ for each sample a on annealing temperature T of Ag-NaCl an studied. The average grain size D could be found condensate. by extrapolating the b*(2θ) dependencies onto S=0 axes as D=1/b*(2θ) at θ=0 (Table 3, Fig. 11). Thus, according to X-Ray data silver is in the nanostate (about 8 nm grain size) in the initial condensate. During heat treatment the grain size becomes larger, the most significantlywith annealing (Fig. 11). It is known that metallic silver can be covered by a thin layer of Ag O oxide in the air atmosphere . However, because of certain limitations for analysis of small quantities of substances, neither X-Ray diffraction method, not TEM found oxygen in Ag-NaCl condensates. Therefore, TGA method was used to study the kinetics of relative change of mass of both porous NaCl condensate, and Ag-NaCl Fig. 11. Silver grain size D in Ag-NaCl condensate at their heating up to 650 °C and condensate, depending on temperature T: 1 – cooling in air. As a result it is shown that the substrate temperature T ; 2 – annealing mass of porous NaCl condensate practically temperature T . an does not change during the experiment (Fig. 12, curve 1), i.e. at electron beam evaporation the salt condenses on the substrate at its stoichiometric composition and does not absorb moisture. Investigations of porous Ag-NaCl condensate performed by TGA method, showed that a slight lowering of its mass occurs in the temperature range of 80 – 120 °C. The 120- 650 °C region is characterized by a slight increase of sample mass (maximum at 360 °C) with its subsequent lowering. At subsequent Fig. 12. Kinetics of relative change of mass cooling and repeated heating-cooling cycles the of NaCl condensate (1) and Ag-NaCl condensate mass does not change (Fig. 12, condensate (2) with differential curve (3) at curve 2). cyclic heating and cooling in air. Considering the data of work , the possibility of formation of an oxide shell on the surface of silver nanoparticles was assessed visually by the colour of deposited condensate. That is, the condensate, in our opinion, gets its hue from the thinnest film of brown-black crystals of the most thermodynamically stable Ag O oxide [24, 25]. Also probable is the presence of Na O, AgOH and AgCl. Then, change of sample mass in the temperature range of 80 – 120 °C can be associated with removal of adsorbed moisture due to decomposition of metastable AgOH phase into oxide and water. A slight increase of sample mass in the temperature range of 250 – Fig. 13. TEM image of Ag-NaCl condensate 360 °C, is associated, apparently, with annealed at 400 °С (1 hour) and rinsed to afteroxidation of sodium oxide (Na O → remove NaCl for 5 days. Ag twins are Na O ) and silver oxide (Ag O → AgO). And, 2 2 2 visible. finally, lowering of sample mass in the temperature range of 340 – 600 °C (430 °C by differential curve 3) is associated with decomposition of AgO oxide into silver and oxygen. This result is in agreement with the data of Roy  on decomposition of AgO oxide at 420 °C (for chemical reactions in aqueous medium values of 200, 250 and 300 °C are given [24, 25]). Fig. 13 shows TEM microstructure of two-phase Ag-NaCl condensate annealed for 1 hour at 400 °C and rinsed to remove NaCl salt for 5 days. One can see that individual silver particles are of a round shape and 8 to 25 nm size. Summing up of the results of the conducted comprehensive study leads to the conclusion that Ag-NaCl condensate deposited on the substrate, contains a mixture of metallic silver nanoparticles (of about 8 nm size and, probably, coated by the thinnest Ag O shell) and Na Ag Cl solid solution. Heat treatment of the initial condensate leads to coagulation and 0.98 0.2 coarsening of Ag particles, as well as precipitation of finest Ag particles from the lattice of solid solution based on sodium chloride. 3.4. Aqueous colloidal solutions of Me+NaCl It is shown that after addition of water to synthesized Me+NaCl condensates, sodium chloride dissolves, and Me nanoparticles, sticking together into aggregates in the form of bundles or chains (Fig. 14), precipitate during sedimentation. (a) (b) Fig. 14. Nanostructure of aggregates of Ag nanoparticles of initial Ag-NaCl condensates (a) and those annealed at 200 °С for 1 hour (b), which were rinsed in distilled water to remove salt. In order to create adsorption layers, preventing particles coarsening as a result of their sticking together, a stabilizer – a surfactant (SA) was added to the colloid. A 1 vol. % aqueous solution of polyvinylpyrrolidone (PVP) was used as SA for silver particles. No agglomeration of silver particles was observed, and the size of silver nanoparticles suspended in SA aqueous solution (determined by DLS method) (Fig. 15), corresponded to the size of nanoparticles in the initial Ag-NaCl porous condensate (about 10 nm). For copper oxide nanoparticles formed in Cu-NaCl condensates 1 vol. % solution of polyvynil alcohol (PVA) was used as SA. Quantitative distribution of particles by sizes, obtained by DLS method (Fig. 16), reveals a maximum at 14-16 nm that corresponds to the size of nanoparticles in porous Cu-NaCl condensate. DLS results are confirmed by electron microscopy studies of Fig. 15. Distribution of particle size in 1 vol.% Fig. 16. Distribution of particle size in 1 vol.% aqueous solution of polyvynilpyrollidone and aqueous solution of polyvynil alcohol and of initial Ag-NaCl condensate. initial Cu-NaCl condensate. (a) (b) Fig. 17. Nanostructure of dried aqueous solution with nanoparticles of silver (а) and copper (b) after rinsing of initial Ag-NaCl (a) and Cu-NaCl (b) condensates to remove salt. dried solutions (Fig. 17). Thus, using colloidal aqueous solutions with SA additives, it was possible to obtain isolated nanoscale particles of silver and copper oxide (Fig. 17). 4. Conclusions Physical synthesis of silver and copper nanoparticles by the method of condensation of mixed molecular beams of metal and salt in vacuum allowed producing nanostructured material in the form of a dry substance (silver and copper nanoparticles in a water-soluble matrix), which enables preservation, storage and transportation of particles for preparation of the required colloidal solutions. Low thermodynamic stability of the compounds of silver with oxygen did not allow their direct identification by TEM and XRD methods, although TGA method provides an indication of the processes of transformation in Ag-O system, and, if we assume that silver nanoparticles have a very thin film of silver oxide in the form of Ag O on their surface , it decomposes at the temperature of 460 °C. Controlling the activity (size) of nanoparticles by varying copper concentration in the condensate, annealing temperature and duration, allows creating various compositions of nanomaterials, based on copper with preset content of the required structural components. List of symbols T – temperature T – melting temperature T – annealing temperature an T – substrate temperature D - grain size a - lattice parameter (period) d – condensate thickness m/m - relative change of mass of TGA B - total isotropic factor R - reliability factor EBPVD - electron-beam physical vapor deposition XRD - X-ray diffraction SEM - scanning electron microscope TEM - transmission electron microscopy DLS - dynamic light scattering EDS - energy-dispersive X-ray spectroscopy TGA - thermogravimetric analyzer SA – surfactant PVP – polyvinylpyrrolidone PVA - polyvynil alcohol References  Sherbakov OB, Korchak GI, Surmacheva OV, Skorokhod IM, Mikhienkova AI (2006) Silver preparations: yesterday, today and tomorrow, Farmatsevticheskii Zhurnal (5): 45-57. http://runonce7531.narod.ru/Z/Ag.pdf  Morones JR, Elechiguerra JL, Camacho A, Holt K, Kouri JB, Ramírez JT, Yacaman MJ (2005) The bactericidal effect of silver nanoparticles, Nanotechnology 16(10): 2346-2353. https://doi.org/10.1088/0957-4484/16/10/059  Shrivastava S, Bera T, Roy A, Singh G, Ramachandrarao P, Dash D (2007) Characterization of enhanced antibacterial effects of novel silver nanoparticles. Nanotechnology 18(22): 225103 (9pp). http://dx.doi.org/10.1088/0957-4484/18/22/225103  Roy R, Hoover MR, Bhalla AS, Slawecki T, Dey S, Cao W, Li J, Bhaskar S (2007) Ultradilute Ag-aquasols with extraordinary bactericidal properties: role of the system Ag- O-H O. Mat Res Innovations 11(1): 3-18. https://doi.org/10.1179/143307507X196167  Alt V, Bechert T, Steinrücke P, Wagener M, Seidel P, Dingeldein E, Scheddin D, Domann E, Schnettler R (2004) Nanoparticulate Silver. A new antimicrobial substance for bone cement. Orthopade 33(8): 885-892. https://doi.org/10.1007/s00132-004-0690-8  Ershov YuA, Pletneva TV (1989) Mechanism of toxic action of inorganic compounds. Moscow, Meditsina. https://www.twirpx.com/look/32693/  Kulskii LA (1987) Silver water. 9th ed., rev. and compl., Kiev, Naukova Dumka, https://www.e-reading.club/bookreader.php/146365/Serebryanaya_voda.pdf  Tilton RC, Rosenberg B (1978) Reversal of the Silver inhibition of Microorganisms by Agar. Applied and Environmental Microbiology 35(6): 1116-1120. https://www.ncbi.nlm.nih.gov/pmc/articles/PMC242993/pdf/aem00221-0134.pdf  Spratt DA, Pratten J, Wilson M, Gulabivala K (2001) An in vitro evaluation of the antimicrobial efficacy of irrigants on biofilms of root canal isolates. Int Endod J 34: 300- https://www.ncbi.nlm.nih.gov/pubmed/11482142  Glushchenko NN (1988) Physico-chemical regularities of biological action of finely dispersed metal powders. Synopsis of Doctor’s thesis, Moscow. https://search.rsl.ru/ru/record/01000129040  Glushchenko NN, Olkhovskaya IP, Pletneva TV, Fatkullina LD, Ershov YuA, Fedorov YuI (1989) Biological impact of highly-dispersed metal powders. Izv AN SSSR, Biological series (3): 415-421. https://elibrary.ru/contents.asp?issueid=1951588  Glushchenko NN, Bogoslovskaya OA, Ol’khovskaya IP (2002) Physicochemical regularities in biological action of highly dispersed powders of metal. Khimicheskaya fizika 21(4): 79-85. https://www.researchgate.net/publication/294711729_Physicochemical_regularities_in_bio logical_action_of_highly_dispersed_powders_of_metals  Borisevich VB (2009) Nanotechnology in veterinary medicine (teaching aid), Edited by Borisevich VB, Borisevich BV, Kaplunenko VG, Kosinov MV, Petrenko OF, Sukhonos VP. Kiev, Comp. «Nanomaterials and nanotechnologies». http://www.4uth.gov.ua/new_books/2009_october.htm nd  Sergeyev GB (2007) Nanochemistry: manual. 2 ed., Moscow University Publ. House. http://padabum.com/d.php?id=122281  Movchan BA (2004) Electron beam technology of evaporation and deposition from the vapour phase of inorganic materials with amorphous, nano- and microstructure, In: Nanosystems, nanomaterials, nanotechnologies (Trans.), Kiev, Akademperiodika 2(4): 1103-1126. http://www.imp.kiev.ua/nanosys/en/articles/index.html  Movchan BA (2006) Inorganic materials and coatings produced by EBPVD. Surface Engineering 22(1): 35-46. https://doi.org/10.1179/174329406X85029  Kurapov YuA, Krushyns’ka LA, Gorchev VF, Kardash MV, Lytvyn SE, Stel’makh YaA, Didikin GG, Romanenko SM, Movchan BO, Chekman IS (2009) Analysis of colloidal systems on the basis of nanoparticles Cu−O−H O and Ag−O−H O obtained by the method 2 2 of molecular beams. Reports of the National Academy of Sciences of Ukraine 7: 176-181. http://dspace.nbuv.gov.ua/handle/123456789/17158  Kurapov YuA, Krushinskaya LA, Litvin SE, Romanenko SM, Stelmakh YaA, Markiev Vya (2014) Production and Thermal Stability of Silver Nanoparticles in the Ag-O System. Powder Metallurgy and Metal Ceramics 53(3-4): 199-204. https://link.springer.com/article/10.1007%2Fs11106-014-9604-4  Checkman IS, Movchan BA, Zagorodnii MI, Gaponov YuV, Kurapov YuA, Krushinskaya LA, Kardash MV (2008) Nanosilver: production technologies, pharmacological properties, indications for use. Mistetstvo likuvannya 5(51): 32-34. http://www.health-medix.com/articles/misteztvo/2008-06-15/32-34.pdf  Lebedev AD, Levchuk YuN, Lomakin AV, Noskin VA (1987) Laser correlation spectroscopy in biology, Kiev, Naukova Dumka. https://search.rsl.ru/ru/record/01001388286  McNeil SE (2001) Characterization of Nanoparticles Intended for Drug Delivery, Humana Press. http://dx.doi.org/10.1007/978-1-60327-198-1  Movchan BA, Demchishin AV (1969) Investigation of the structure and properties of thick vacuum condensates of nickel, titanium, tungsten, aluminium oxide and zirconium oxide. The Physics of Metals and Metallography, 28(4): 653-660. http://impo.imp.uran.ru/fmm/electron/vol28_4/abstract10.pdf  Kovinsky IS, Krushinskaya LA, Movchan BA (2011) Structure and some properties of sodium chloride condensates produced by electron beam evaporation with next deposition in vacuum. Advances in Electrometallurgy 9(1): 42-46. https://patonpublishinghouse.com/sem/pdf/2011/sem201101all.pdf  Rabinovich VA, Khavin Zya (1991) Brief chemical reference book, Leningrad, Khimia, 103-104. http://booktech.ru/books/himiya/810-kratkiy-himicheskiy-spravochnik-1991-va- rabinovich.html  Stepin BD, Tsvetkov AA (1994) Inorganic chemistry, Мoscow, Vysch. shk., 400-401. http://www.alleng.ru/d/chem/chem195.htm
Condensed Matter – arXiv (Cornell University)
Published: Jun 14, 2018
Access the full text.
Sign up today, get DeepDyve free for 14 days.